# effect of covalent functionalization on young’s modulus rbatra/pdfpapers/book_chapter...effect of...

Post on 14-May-2018

214 views

Embed Size (px)

TRANSCRIPT

Effect of Covalent Functionalizationon Youngs Modulus of a Single-WallCarbon Nanotube

Priyal H. Shah and Romesh C. Batra

Abstract Effective utilization of carbon nanotubes (CNTs) as reinforcements incomposites necessitates good interfacial bonding with the surround matrix mate-rial. The covalent functionalization of CNTs is an effective method to enhance thisbonding. However, covalent bonds introduced by a functional group may alter thepristine structure of the CNT and lower its mechanical properties. Here we studythe effect of hydrogen (H), hydroxyl (OH), carboxyl (COOH), and amine(NH2) functionalization on Youngs modulus of a single-wall CNT (SWCNT)using molecular mechanics (MM) simulations with the MM3 potential and thesoftware TINKER. Both pristine and functionalized SWCNTs have been deformedin simple tension. From the strain energy of deformation vs. the axial strain curves,the value of Youngs modulus has been derived as a function of the functionali-zation group and the amount of functionalization. It is found that Youngs modulusdecreases by about 30 % with 20 % of functionalization, the reduction is essen-tially proportional to the increase in the percentage of the functionalizationmaterial and is nearly the same for each of the four functional groups studied.

Keywords Carbon nanotubes Youngs modulus Functionalization Molecularmechanics Virtual tension test

P. H. Shah R. C. Batra (&)Department of Engineering Science and Mechanics, Virginia Polytechnic Instituteand State University, Blacksburg, VA 24061, USAe-mail: rbatra@exchange.vt.edu

P. H. Shahe-mail: spriyal@vt.edu

K. I. Tserpes and N. Silvestre (eds.), Modeling of Carbon Nanotubes, Grapheneand their Composites, Springer Series in Materials Science 188,DOI: 10.1007/978-3-319-01201-8_4, Springer International Publishing Switzerland 2014

111

1 Introduction

Researchers have employed experimental, analytical, density functional theory(DFT), molecular dynamics (MD) and molecular mechanics (MM) simulations topredict mechanical properties of carbon nanotubes (CNTs). Assuming that the wallthickness of a single-wall CNT (SWCNT) can be approximated as 0.34 nm, Treacyet al. (1996), Wong et al. (1997), and Krishnan et al. (1998) experimentallydetermined that Youngs modulus of a CNT is in terapascal (TPa) range. Xing et al.(2004) employed MD simulations to predict Youngs modulus of a SWCNT. Li andChou (2003) computed elastic properties of CNTs using a combined structuralmechanics and MM approach. Chang and Gao (2003) investigated size dependentelastic properties of SWCNTs through MM simulations. Sears and Batra (2004)determined the wall thickness, Youngs modulus, and Poissons ratio of CNTsusing MM simulation with the MM3 potential and the software TINKER. Theyassumed that the response of a SWCNT in simple tension is energetically equiv-alent to that of a thin cylinder made of an isotropic and homogeneous material.Furthermore, the wall thickness of the cylinder equals that of the SWCNT. Theyfound the wall thickness and Youngs modulus of a SWCNT to be 0.046 nm and7.26 TPa, respectively. Shen and Li (2004) used MM potential and energy equiv-alent principle to determine values of five elastic constants of a CNT assuming theCNT as a transversely isotropic material with the centroidal axis of the tube as theaxis of transverse isotropy. Batra and Sears (2007) proposed that the axis oftransverse isotropy of a CNT is a radial line rather than the centroidal axis. Bystudying with the MM simulations radial expansion of a SWCNT, they showed thatYoungs modulus in the radial direction is about 1/4th of that in the axial direction.Gupta and Batra (2008), Batra and Gupta (2008) predicted the wall thickness andthe material moduli of a SWCNT by matching frequencies of bending, axial andtorsional vibrations as well as that of radial breathing modes of a freefree SWCNTwith those of the continuous cylinder of the same length and mean radius as theSWCNT. Wu et al. (2008) developed an atomistic based finite deformation shelltheory for a SWCNT and found its stiffness in tension, bending, and torsion.

The SWCNTs due to their cylindrical shape, large length to diameter ratio, andhigh specific properties are potential candidates as reinforcements in composites.However, the effectiveness of SWCNTs as reinforcements depends on their uni-form dispersion in and strong adhesion with the surrounding matrix. It has beenvery challenging to simultaneously meet these two requirements. The function-alization of SWCNTs appears to be an effective means of achieving good bondingbetween SWCNTs and the surrounding matrix. The surface properties of CNTscan be modified by either physical or chemical functionalization. The physicalfunctionalization is achieved by attaching noncovalent groups, such as polymer,peptides or surfactants to the nanotubes. It is advantageous since it does not alterthe pristine structure of nanotubes hence the mechanical properties of CNTs arenot affected. However, these functional groups are attached to nanotubes withweak van der Waals interactions resulting in low load transfer efficiency between

112 P. H. Shah and R. C. Batra

the nanotube and the matrix. In comparison, the chemical functionalizationinvolving the covalent attachment of functional groups to atoms of CNTs providesrelatively strong interfacial bonding between CNTs and the surrounding matrixthereby enhancing the load transfer efficiency. Haddon et al. used the nanotube-bound carboxylic acid groups for attaching long alkyl chains to SWCNTs viaamide linkages (Chen et al. 1998; Hamon et al. 1999; Niyogi et al. 2001) and viacarboxylate-ammonium salt ionic interactions (Chen et al. 2001). Khare et al.(2002) developed hydrogenated CNTs using electric discharge. Sun et al. showedthat the esterification of the carboxylic acid groups could also be used to func-tionalize and solubilize nanotubes of any length (Riggs et al. 2000; Sun et al. 2001;Fu et al. 2001). Wilson et al. illustrated the use of anilines to functionalizenanotubes (Sun et al. 2001). Grujicic et al. (2006) investigated the effect ofcovalent functionalization of triple-walled CNTs on the efficiency of matrix-nanotube load transfer. Their results reveal that the covalent functionalizationimproves the load transfer efficiency especially when loads are applied in adirection orthogonal to the axis of the CNT. Experimental works (Cooper et al.2002; Barber et al. 2003; Shofner et al. 2006; Buffa et al. 2007; Sun et al. 2008)have demonstrated the effectiveness of covalent functionalization in increasing theinterfacial bonding strength between CNTs and polymer chains.

Although chemical functionalization is effective in enhancing the binding ofCNTs with the surrounding matrix, it may damage the pristine structure of a CNTdue to the introduction of covalent bonds, and reduce the mechanical stiffness ofthe CNT. Much of the research work dealing with the determination of Youngsmodulus and other elastic properties of CNTs has considered pristine CNTs. Sincethe covalently functionalized CNTs would be better candidates for reinforcementsin a composite than the pristine CNTs, it is important to determine the effect ofcovalent functionalization on Youngs modulus of a CNT. Zhang et al. (2008) usedatomistic simulations to analyze mechanical properties of hydrogenated SWCNTsand found a decrease in Youngs modulus, strength, and ductility of the CNTs withan increase in the percentage of CH bonds. Kuang and He (2009) computedYoungs moduli of vinyl functionalized SWCNTs using MM simulations with thecondense-phase optimized molecular potential for atomistic simulation studies(COMPASS) force field and found that Youngs modulus depends on the densityof the sp3 hybridized carbon atoms and chirality of the CNTs. Up to 33 %reduction in Youngs modulus was observed in their study with 38 % content ofthe functionalizing material. Ling et al. (2012) predicted Youngs modulus offunctionalized CNTs using MM and MD simulations with the COMPASS forcefield and observed that Youngs modulus depends on the type of functionalizingmaterial and the amount of functionalization. Recently, Milowska and Majewski(2013) studied effect of different functional groups on elastic properties of func-tionalized CNTs using DFT calculations. Their results showed that an increase inamount of covalently bound material to the wall of a CNT decreases Youngs,shear and bulk moduli. Here we have considered four functional groups namely,hydrogen (H), hydroxyl (OH), carboxyl (COOH), and amine (NH2) andcompared their effects on the modulus of elasticity of a SWCNT with varying

Effect of Covalent Functionalization on Youngs Modulus 113

percentage of functionalization. The study has been carried out using MM simu-lations with the freely available software TINKER (Ponder 2000).

2 Molecular Mechanics Simulations

2.1 Force-Field

The MM3 potential (Allinger et al. 1989) with higher order expansions and cross-terms has been used to model interatomic interactions. This potential is suitable forstudying deformations of CNTs because of similarities between sp2 bonds in thehexagonal structure of CNTs and the hexagonal structure of aromatic proteins forwhich the potential was originally developed. This potential describes the energyof the system as summation of the energies due to bonded and non-bondedinteractions. The contributions for bonded interactions come from bond stretchingUs; in-plane angle bending Uh; out of plane bending Uc; torsion U/; andcross-interactions including stretch-bend Usb; angleangle Uhh0 and stretch-torsion Us/. The non-bonded interactions are van der Waals UvdW and dipoledipole electrostatic Ull0 . Equation (1) gives expressions for these energies.

Us 71:94Ksr r021 2:55r r0 7

122:552r r02

Uh 0:0219Khh h02 1 0:014h h0 5:6105h h02

7